Crystallographic Characterization of Lu2C2n (2n = 76-90): Cluster Selection by Cage Size
Lu, Xing; Shen, Wangqiang; Bao, Lipiao; Hu, Shuaifeng; Yang, Le; Jin, Peng; Xie, Yun-Peng; Akasaka, Takeshi; Chemical Science  (2019) –; doi:10.1039/C8SC03886D

data_1550156
_publ_section_title
;
 Crystallographic Characterization of Lu2C2n (2n = 76-90): Cluster
 Selection by Cage Size
;
_journal_name_full               'Chemical Science'
_journal_paper_doi               10.1039/C8SC03886D
_journal_year                    2019
_chemical_formula_moiety         'Lu2 C84, C36 H44 N4 Ni, C6 H6 '
_chemical_formula_sum            'C126 H50 Lu2 N4 Ni'
_chemical_formula_weight         2028.35
_chemical_name_common            'Lu2@C2v-C84 Ni(OEP)'
_chemical_name_systematic        'Lu2@C2v-C84 Ni(OEP)'
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2017-10-26 deposited with the CCDC.
2018-10-29 downloaded from the CCDC.
;
_cell_angle_alpha                90.000(5)
_cell_angle_beta                 94.510(5)
_cell_angle_gamma                90.000(5)
_cell_formula_units_Z            4
_cell_length_a                   25.410(5)
_cell_length_b                   15.110(5)
_cell_length_c                   19.917(5)
_cell_measurement_reflns_used    9835
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      23.133
_cell_measurement_theta_min      2.325
_cell_volume                     7623(4)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.974
_diffrn_measured_fraction_theta_max 0.974
_diffrn_measurement_device_type  'CCD MX300-HE'
_diffrn_measurement_method       'phi scans'
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.6525
_diffrn_reflns_av_R_equivalents  0.0504
_diffrn_reflns_av_unetI/netI     0.0303
_diffrn_reflns_Laue_measured_fraction_full 0.974
_diffrn_reflns_Laue_measured_fraction_max 0.974
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -29
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            51276
_diffrn_reflns_point_group_measured_fraction_full 0.974
_diffrn_reflns_point_group_measured_fraction_max 0.974
_diffrn_reflns_theta_full        23.048
_diffrn_reflns_theta_max         23.133
_diffrn_reflns_theta_min         1.687
_diffrn_source                   'SSRF, Beamline BL17B'
_exptl_absorpt_coefficient_mu    2.339
_exptl_absorpt_correction_T_max  0.7449
_exptl_absorpt_correction_T_min  0.5218
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    1.767
_exptl_crystal_description       Block
_exptl_crystal_F_000             4016
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.080
_exptl_crystal_size_min          0.070
_refine_diff_density_max         1.015
_refine_diff_density_min         -1.434
_refine_diff_density_rms         0.118
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.068
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     866
_refine_ls_number_reflns         7072
_refine_ls_number_restraints     864
_refine_ls_restrained_S_all      1.131
_refine_ls_R_factor_all          0.0890
_refine_ls_R_factor_gt           0.0818
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1486P)^2^+43.3856P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2353
_refine_ls_wR_factor_ref         0.2438
_reflns_Friedel_coverage         0.000
_reflns_number_gt                6280
_reflns_number_total             7072
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8sc03886d2.cif
_cod_data_source_block           Lu2@C2v-C84
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_database_code               1550156
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.799
_shelx_estimated_absorpt_t_max   0.849
_shelx_res_checksum              85534
_shelx_fab_checksum              60205